Active Standard ASTM D635 | Developed by Subcommittee: D20.30
Book of Standards Volume: 08.01
Historical (view previous versions of standard)
Significance and Use
Tests made on a material under conditions herein prescribed are of value in comparing the rate of burning or extent and time of burning characteristics, or both, of different materials, in controlling manufacturing processes, or as a measure of deterioration or change in these burning characteristics prior to or during use. Correlation with flammability under actual use conditions is not implied.
The rate of burning and other burning phenomena will be affected by such factors as density, pigments, any anisotropy of the material and the thickness of the specimen. Test data shall be compared only for specimens of similar thickness, whether comparisons are being made with the same or different materials. The rate of burning and other burning phenomena will vary with thickness.
It is feasible that sheet materials that have been stretched during processing will relax during burning and give erratic results unless they are first heated above their deflection temperature, in accordance with Test Method D648, for a time sufficient to permit complete relaxation.
Burning tests require that certain variables be arbitrarily fixed, for example, specimen size, energy source and application time, and end points. Materials will be found that are unusually sensitive to one or more of the conditions chosen for this method leading to highly variable results. Additional burning characterization by other methods is highly desirable in such cases (see Note 2).
In this procedure, the specimens are subjected to specific laboratory test conditions. If different test conditions are substituted or the end-use conditions are changed, it will not always be possible by or from this test to predict changes in the fire-test-response characteristics measured. Therefore, the results are valid only for the fire-test-exposure conditions described in this procedure.
1.1 This fire-test-response test method covers a small-scale laboratory screening procedure for comparing the relative linear rate of burning or extent and time of burning, or both, of plastics in the form of bars, molded or cut from sheets, plates, or panels, and tested in the horizontal position.
Note 1—This test method, and test method A of IEC 60695-11-10 are technically equivalent.
Note 2—For additional information on materials which do not burn to the first reference mark by this test, see Test Method D3801.
1.2 This test method was developed for polymeric materials used for parts in devices and appliances. The results are intended to serve as a preliminary indication of their acceptability with respect to flammability for a particular application. The final acceptance of the material is dependent upon its use in complete equipment that conforms with the standard applicable to such equipment.
1.3 The classification system described in Appendix X1 is intended for quality assurance and the preselection of component materials for products.
1.4 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.5 This standard is used to measure and describe the response of materials, products, or assemblies to heat and flame under controlled conditions, but does not by itself incorporate all factors required for fire hazards or fire risk assessment of materials, products, or assemblies under actual fire conditions.
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. For specific hazards statements, see 9.2.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D618 Practice for Conditioning Plastics for Testing
D648 Test Method for Deflection Temperature of Plastics Under Flexural Load in the Edgewise Position
D883 Terminology Relating to Plastics
D1929 Test Method for Determining Ignition Temperature of Plastics
D2843 Test Method for Density of Smoke from the Burning or Decomposition of Plastics
D3801 Test Method for Measuring the Comparative Burning Characteristics of Solid Plastics in a Vertical Position
D5025 Specification for Laboratory Burner Used for Small-Scale Burning Tests on Plastic Materials
D5207 Practice for Confirmation of 20-mm (50-W) and 125-mm (500-W) Test Flames for Small-Scale Burning Tests on Plastic Materials
E84 Test Method for Surface Burning Characteristics of Building Materials
E176 Terminology of Fire Standards
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
IEC StandardsIEC 60695-11-10 Fire Hazard Testing--Part 11-10 Test Flames--50W Horizontal and Vertical Flame Test Methods
ICS Number Code 13.220.40 (Ignitability and burning behaviour of materials and products); 83.080.01 (Plastics in general)
UNSPSC Code 13100000(Rubber and elastomers)